## EFFECT OF THE TECHNIQIE OF DRAWING WITH SHEAR ON THE STRUCTURE AND THE PROPERTIES OF LOW-CARBON WIRES

Donetsk Institute for Physics and Engineering named after А.А. Galkin NAS of Ukraine 72 R.Luxemburg Str., 83114, Donetsk, Ukraine

1 SPA «Donix», Donetsk, Ukraine

To obtain  the  materials  of  ultrafine  grain  (UFG)  structure,  different  methods  of  severe  plastic deformation (SPD) with shear in both cold and hot state are used: equal-channel angular pressing, twist extrusion, and combination of these methods with succeeding rolling, upset, drawing etc. The application  of  these  methods  allows  substantial  increase  in  the  strength  of  the  material  at  certain conserved reserve of plasticity.

However  the  mentioned  combination  of  the  methods  can  not  be  realized  at  wiredrawing production  plants, whereas  the last are very interested in new  technological  and  operation characteristics of long-length wire products [1,2]. One of constraints  imposed upon the production of UFG wire is that the total output of the materilas  produced by the listed SPD methods is measured by tens of kilograms and tons but the required capacity  of wiredrawing production is hundreds of thousand tons.

A possible solution of the problem of the long wire products can be application of drawing with shear. As may be supposed, an increase in the plasticity reserve of rods and wires allows cheapening and simplification of the production technique due to the abandonment of the intermediate anneal.

In [1-9],  different methods  of  severe  plastic  deformation  of  long  metal  billets  of  varied configuration are described. The works [5,6,9] are of special interest here.

The  authors  of  [5]  analyze  the  application  of  sign-alternation  twisting  of  cold-drawn  furniture without  an  additional  heating.  The  main  advantages  of  the  method  are  continuous  operation  and possible application to the production of long products with enhanced mechanical properties. In [6], a method of plastic structure formation  in the  material of  long  billets  is  tested,  and  a  facility  of  the realization  is  presented  that  is  based  on  sign-alternating  deformation  within  intersecting  channels. The deformation zone is formed within the billet due to a shift of the symmetry axes of the channels combined with uniaxial tension. The presented method is intermittent, and the finite billets of several meters in length can be produced. The advantage of the method is formation of a fine grain structure. But the deforming block is even more complex than that in the case of [5]. Both the methods [5,6] do not permit production of the wire of small diameter.

A drawing-based method of obtaining of UFG structure in long products is described in [9]. The main  advantage  is  continuous  operation  and  possible  application  to  the large-scale drawing production. A drawback is labor intensity of drawing because a complex technical facility is used that requires disassembling and new installation in the course of replacement of wire drawing dies.

The present paper reports the developed technique of drawing with shear aimed at enhancement of technological  plasticity  of  low-carbon  steels  without  thermal  treatment.  The  technology  should provide definite physical and mechanical properties of the wire. It also should be cheap, simple and reliable in the course of operation.

3.9

5.0

5.3

## Experimental technique

The experiment was carried out with using the billet of steel ER70S-6 (Table 1). The drawing was realized at the plant АZТМ 7000/1 by the developed (experimental) technique (with shear dies) and by the classical one (with the standard round dies). The drawing routes of the both techniques are listed in Table 2.

Тable 1

Chemical composition of ER70S-6  steel, %

| C       | Mn      | Si       | S     | P     | Cr     | Ni    | Cu    | N      |
|---------|---------|----------|-------|-------|--------|-------|-------|--------|
| 0.071   | 1.98    | 0.84     | 0.015 | 0.018 | 0.015  | 0.009 | 0.016 | 0.0055 |
| Ti      | As      | B        | Al    | V     | Mo     | W     | Co    |        |
| < 0.005 | < 0.005 | < 0.0005 | 0.005 | 0.006 | < 0.01 | 0.024 | 0.01  |        |

Тable 2 Drawing routes for the wires produced by the experimental and the standard techniques

| Technique    | Die diameter, mm   | Die diameter, mm   | Die diameter, mm   | Die diameter, mm   | Die diameter, mm   | Die diameter, mm   | Die diameter, mm   | Die diameter, mm   | Die diameter, mm   | Die diameter, mm   |
|--------------|--------------------|--------------------|--------------------|--------------------|--------------------|--------------------|--------------------|--------------------|--------------------|--------------------|
| Experimental | 6.15               | 5.4                | 5.2 *              | 5.0                | 4.30               | 3.90               | 3.5                | 3.06               | 2.70               | 2.39               |
| Conventional |                    |                    | 5.30               |                    |                    |                    |                    |                    |                    |                    |

Note . * - die with shear

The  obtained  samples  from  6.15  tо  3.90  mm  in  diameter  were  subjected  to  mechanical  tests,  in particular, the ultimate tension strength and the contraction ratio were measured (Fig. 1).

The microstructures of the annealed sample and the deformed ones were studied at the 100-1000 power  device  «Neophot-32»  after  repetitive  polishing  and    etching  of  the  grain  boundaries  (the composition of the etching agent: 4% nitric acid, 97% alcohol). The photos were made by the optical microscope Axiovert 40 MAT.

0.8

824 838

766 807

2

0.6

6 0.2

642 642

Wire diameter, mm

6.15

а

Fig.  1. Mechanical  properties  of  the  ER70S-6  steel  wire  obtained  by  the  conventional  ( ■ ) and    the experimental ( ) technique: а - the ultimate tensile strength σ uts , b - the contraction ratio 

![image](https://ac.marcodsn.me/arxiv-markdown-images/1408.0125v1-figure-e6893279-9f01-4f95-9cb6-1ac5a7b337d6.jpg)

Тable 3

## Elongation ratio k of the  ER70S-6 wire

| Technique    | k       | k       | k     |
|--------------|---------|---------|-------|
|              |  6.5  |  5.0  |  3.9 |
| Experimental | 1       | 0.35    | 0.19  |
| Conventional |         | 0.21    | 0.10  |

The  estimation  of  the  grain  size  and  the  fragment  size  was  performed  in  the  transversal  and longitudinal directions of the samples. 100 measurements were made on every photo. The elongation ratio was calculated as

$$k = D _ { 1 } / D _ { 2 },$$

where D 1, D 2 were the lengths of the grain along the grain elongation and in the cross-section of the sample, respectively, mm.

Besides,  Vickers  hardness  HV  (loading  of  200  g)  and  microhardness H μ  (loading  of  100  g)  were measured. The measurement error was  5%. The density of the  samples was  measured by  hydrostatic weighing. Strength tests were carried out with using UММ-50 test machine at the temperature of 293 K and the rate of loading of 10 mm/min according to GOST 25.601-80.

## Experiment results

The tests have demonstrated that when the diameter of the sample is reduced, the ultimate tensile strength remains at the same level irrespective of the conventional or experimental technique   (Fig. 1, а ),  and  the  contraction  ratio  of  the  sample  processed  by  the  experimental  technique  is  higher  as compared to the conventional drawing  (Fig. 1, b ).

On the basis of the  mean  values,  it  is  seen  that the  reduction  of  the  diameter  after the  conventional technique  is  associated  with  the  increase  in  the  ultimate  tensile  strength  by  380  N/mm ,  and  the 2 experimental technique yields 240 N/mm . 2

After the conventional technique, the value of the contraction ratio is substantially decreased from 69 to 28%, and the drop after the experimental technique is from 69 to 55%.

One  of  the  distinguishing  features  of  the  experimental  technique  is  a  decrease  in  the  structure anisotropy  in  the  longitudinal  samples.  An  evidence  of  the  fact  is  an  increase  in  the  elongation  ratio (Table 3). The photos of microstructures confirm the calculated data (Fig. 2).

![image](https://ac.marcodsn.me/arxiv-markdown-images/1408.0125v1-figure-1d408de8-b9af-4255-a715-bb654d4182d8.jpg)

а

Fig. 2. Microstructure of the samples of the wire of ER70S-6  5.0 obtained by the experimental technique ( а ) and the conventional technique ( b ),  100. The scale represents 10 μm

![image](https://ac.marcodsn.me/arxiv-markdown-images/1408.0125v1-figure-26c3e797-134b-4215-a1cf-a03e4a87629f.jpg)

The analysis of the structures revealed the following principal structure features.

1. The etchability of perlite colonies is higher at the conventional technique that is related to nonequilibrium of perlite after drawing. In the longitudinal section, along the section at the conventional technology is larger that of the experimental technique.

- 2. It has been established that the experimental technique results in decreased anisotropy of the grains, and the grain size is reduced as a whole, when the degree of deformation increases. But at certain stages, successive decrease and increase in the grain size is observed that is supposed to be related  to  the  progress  in  competitive  processes  of  fragmentation  and  dynamical  polygonization.

For instance, in the tested samples of  5.2 and  5.0 in cross-section, the structure is enlarged: the ferrite  grains  and  the  sizes  of  perlite  colonies  grow  as  compared  to  the  sample  of  6.15.  In  the cross-section of the experimental sample,  the structure was larger in comparison with the sample obtained  by  the  conventional  technique.  The  structure  of  the  last  sample  contained  more  perlite phase.

- 3. In the cross-section of the samples of  3.9 obtained by the conventional technique, there is a surface  zone  of  about    200-300  m    that  differs  in  etchability.  This  effect  is  not  found  after  the experimental  technique,  the  metal  is  homogeneous,  the  ferrite  grains  are  lager,  the  size  and  the amount of perlite is much less than that after the conventional technique.
- 4. The samples of  2.39 by the conventional technique are etched better, so, the degree of nonequilibrium is higher. In the longitudinal section of the conventional samples, the anisotropy is more intensive, the ferrite grains are smaller, the perlite colonies are elongated as stripes (Fig. 3). The same effect is observed in the cross-section. Besides, healing of  pores and microcracks is registered in the course of the experimental drawing   (compare Fig. 3, c and d ).

## Conclusions

- 1.  The application of the experimental dies allows improvement of the mechanical properties of the  samples  when  the  diameter  is  decreased  after  drawing:  the  contraction  ratio  of  the  wire  is insignificantly reduced and stays at a relatively high level as compared to the conventional technique where the contraction ratio is halved.
- 2.  The  use  of  the  experimental  technique  permits  variation  of  the  ferrite  grain  size  (successive increase  and  decrease)  in  comparison  with  the  conventional  technique  where  the  increase  in  the degree of deformation results in unambiguous grain reduction.
- 3.  The  application  of  the  experimental  technique  generates  pore  healing  in  the  wire  of  a  small diameter.

![image](https://ac.marcodsn.me/arxiv-markdown-images/1408.0125v1-figure-cea9e4af-4e97-44de-b30d-cd9457d896f9.jpg)

![image](https://ac.marcodsn.me/arxiv-markdown-images/1408.0125v1-figure-3de252a0-6ff3-441a-b6e5-598b57201785.jpg)

а

![image](https://ac.marcodsn.me/arxiv-markdown-images/1408.0125v1-figure-e0f04ed5-6329-466e-8e4e-fc974cfd9381.jpg)

b

![image](https://ac.marcodsn.me/arxiv-markdown-images/1408.0125v1-figure-d215cda8-4fc0-46bd-81ec-ff8079097b65.jpg)

- Fig.  3. Microstructure  of  the  central  zone  of  the  ER70S-6    wire  samples  of  2.39  obtained  by  th4e conventional technique ( a , c )  and  by  the  experimental technique ( b,  d )  : а , b -  the  cross-section, c,  d -  the longitudinal section,  100. The scale is as in Fig. 2
- 4. To prevent the heating of the wire and the die, it is necessary to pass to the experimental drawing through two experimental dies with shear separated by a standard die. This configuration will result in enhanced fabricability and reduction of the drawing force.
- 1. E. Astafurova, G. Zakharova., E. Naydenkin., G. Raab., P. Odesskiy., S. Dobatkin , Materials letters 1. #4, 198 (2011).
- 2. E. Astafurova, G. Zakharova, E. Naydenkin, S. Dobatkin, G. Raab, FMM 110 , 275 (2010).
- 3. N. Kolbasnikov, O. Zotov., V.Duranichev, Metall treatment  # 4, 25 (2009). ,
- 4. S. Yakovleva, S. Makharova, News of Samarian scientific centre of RAS, 12 , # 1(2), 589 (2010).
- 5. E. Kireev, M. Shulyak, A. Stolyarov, Steel # 3, 56 (2009).
- 6. Patent RF # 2440865, The method of structure of plastic material of long workpieces and device for its implementation, A. Matveev, R. Kazakov, Yu. Shumkina, V. Kurganskiy, application # 2010121631/02, 27.05.2010.
- 7. E. Astafurova, G. Zakharova., E. Naydenkin., G. Raab., S. Dobatkin Е.Г. , Астафурова, Physical mesomechanic 13 , № 4, 91 (2010).
- 8. A.  Zakirova,  R.  Zaripova,  V.  Semenov, News  UGATU,  Engineering,  materials  science  and  thermal processing of metals 11 , № 2 (29), 123 (2008).
- 9. Patent  RF  # 2347633,  A  method  for  producing  ultrafine  semis  drawing  shift,  G.  Raab,  A.  Raab, application # 2007141899/02, 12.11.2007.
E. G. Pashinskaya V. N. Varyukhin A. A. Maksakova A. I. Maksakov1 A. A. Tolpa1 A. V. Zavdoveev
Effect of the techniqie of drawing with shear on the structure and the properties of low-carbon wires
The technology of drawing with shear is developed. It allows increasing
technological plasticity of low carbon steel without heat treatment. It is
found that the use of experimental technology can improve mechanical properties
of wire samples with the diameter reduced during drawing: the relative
reduction of the wire decreases slightly and remains at high level compared
with the classical technology, where the relative reduction in the course of
drawing drops more than twice. It is shown that the use of experimental
technology allows varying the size of a ferrite grain (increase or decrease)
compared with the classical technology, where increasing of deformation degree
results in grain reduction. Furthermore, the experimental technology allows
reducing the number of pores in a wire of small diameter. To prevent heating of
the wire and the drawing dies, it is proposed to use experimental drawing
through two experimental dies with shear separated by an ordinary die. As a
result, the workability of the process will be enhanced and the efforts of
drawing will be reduced.